DOI: 10.17188/1747418
title: Materials Data on Li5V3P8O29 by Materials Project

description: Li5V3P8O29 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are ten inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 66–70°. There are a spread of Li–O bond distances ranging from 1.86–2.28 Å. In the second Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.29 Å. In the third Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share a cornercorner with one LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.97–2.26 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.96–2.15 Å. In the fifth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.19 Å. In the sixth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.90–2.15 Å. In the seventh Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.86–2.43 Å. In the eighth Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.91–2.21 Å. In the ninth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share a cornercorner with one LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 2.00–2.22 Å. In the tenth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.91–2.74 Å. There are six inequivalent V+4.33+ sites. In the first V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.88–2.00 Å. In the second V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–2.00 Å. In the third V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.88–2.01 Å. In the fourth V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.84–2.03 Å. In the fifth V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.84–2.04 Å. In the sixth V+4.33+ site, V+4.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.87–2.04 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–46°. There are a spread of P–O bond distances ranging from 1.48–1.62 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–47°. There are a spread of P–O bond distances ranging from 1.49–1.61 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 44–47°. There are a spread of P–O bond distances ranging from 1.49–1.63 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 25–34°. There are a spread of P–O bond distances ranging from 1.49–1.59 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–37°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 40–49°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–37°. There are a spread of P–O bond distances ranging from 1.49–1.61 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 40–48°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–43°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–45°. There are a spread of P–O bond distances ranging from 1.49–1.62 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 39–44°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 28–36°. There are a spread of P–O bond distances ranging from 1.49–1.60 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–37°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 39–40°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–40°. There are a spread of P–O bond distances ranging from 1.51–1.63 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–46°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. There are fifty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 150 degrees geometry to one Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the third O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Li1+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a trigonal planar geometry to two Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted linear geometry to one Li1+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.33+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+4.33+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a trigonal planar geometry to two Li1+ and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V+4.33+ and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V+4.33+, and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twenty-eighth O2- site, O2- is bonded in a distorte